Journal of Power Sources 269 (2014) 111e116
Contents lists available at ScienceDirect
Journal of Power Sources journal homepage: www.elsevier.com/locate/jpowsour
Key parameters in design of lithium sulfur batteries Ning Ding a, Sheau Wei Chien a, T.S. Andy Hor a, b, Zhaolin Liu a, *, Yun Zong a, * a
Institute of Materials Research and Engineering (IMRE), A*STAR (Agency for Science, Technology and Research), 3 Research Link, Singapore 117602, Republic of Singapore b Department of Chemistry, National University of Singapore, 3 Science Drive 3, Singapore 117543, Republic of Singapore
h i g h l i g h t s
g r a p h i c a l a b s t r a c t
Studied the effect of the carbon to sulfur ratio on the performance of LieS batteries. Investigated the inﬂuence of sulfur loading density and electrolyte volume on cell capacity. Provided a guideline for the design of high performance LieS batteries.
a r t i c l e i n f o
a b s t r a c t
Article history: Received 21 May 2014 Received in revised form 25 June 2014 Accepted 1 July 2014 Available online 9 July 2014
In this paper, we discuss some key parameters in design of lithium sulfur batteries with high energy density, in particular carbon/sulfur ratio, sulfur loading density, electrolyte volume and electrode deformability, which directly impact the battery performance in terms of capacity, cycleability, and processibilities, etc. We ﬁnd that a carbon to sulfur ratio of 1:2 (w/w) in the electrode is good for high speciﬁc capacity, giving a capacity of 538 mA h g1 which is 3 times as high as that of LiCoO2 cathode. The issue of fragileness for electrode at high sulfur loading density is mitigated by replacing carbon black with ﬁne graphite powders. With these optimizations the carbonesulfur electrode gives an energy density of 5.88 mW h cm2 which corresponds to 60% of that of the commercial LiCoO2 electrode. © 2014 Elsevier B.V. All rights reserved.
Keywords: Lithium sulfur battery Carbon to sulfur ratio Sulfur loading density Electrolyte volume Deformability
1. Introduction Lithium-ion (Li-ion) batteries have dominated the power supply market of portable electronic devices since the ﬁrst launch of commercial lithium cobalt oxide/carbon (LiCoO2/C) cells by Sony in 1991. Though being widely used the Li-ion batteries are seeing their bottlenecks in energy density limited by the lithium capability of lithium transition metal oxide (Li-M-O, M ¼ Ni, Co and Mn) cathodes which typically deliver a theoretical speciﬁc capacity in the
* Corresponding authors. E-mail addresses: [email protected]
(Z. Liu), [email protected]
(Y. Zong). http://dx.doi.org/10.1016/j.jpowsour.2014.07.008 0378-7753/© 2014 Elsevier B.V. All rights reserved.
range of 120e320 mA h g1 [1,2]. To meet the ever-growing demands on rechargeable batteries with higher energy density, nonlithium intercalated transition metal oxides, such as MexOy (Me ¼ V [3e5] or Cr ) and group 16 (VIA) elements (primarily oxygen , sulfur and selenium ), have recently been exploited as the cathode materials for next-generation lithium batteries. For these non-lithium intercalated cathodes, lithium is used as the counter anode. In this case extra care in safety is required, as the growth of dendrites may cause short-circuit and explosion if the electrode is not properly engineered. Lithiumesulfur (LieS) system is considered as the safest among batteries using lithium metal as anode, as its discharged products, lithium polysulﬁdes, are soluble in the electrolyte that signiﬁcantly suppress the formation of lithium dendrites . LieS battery is also a choice for its high energy
N. Ding et al. / Journal of Power Sources 269 (2014) 111e116
density. Theoretically, sulfur can deliver a speciﬁc capacity of 1672 mA h per gram sulfur (mA h g1-sulfur) that is nearly 5 times as high as that of Li-ion batteries . Furthermore, LieS battery is a cost-effective choice, as sulfur is obtained from the byproducts of oil reﬁning with the annual world production of 69 million tons (Mt) in 2011  which is sufﬁcient for 4 billions of 60 kW automobiles. So far, major efforts in the LieS battery research have been the development of sulfur composites with various microstructures for the cathode, and some interesting ﬁndings were reported [13e23]. For sulfur cathode, one has to deal with its poor intrinsic electrical conductivity (1 1015 S m1) by incorporating large portion of carbon black, which lowers the sulfur content and reduces the gravimetric and volumetric energy density at cell level . High sulfur content (up to 70 wt%) can be achieved by incorporating sulfur into highly ordered mesoporous carbon, followed by coating with polyethylene glycol , or using a lower load of graphene or carbon nanotubes as substitute of carbon black [26e30]. More recently, the concept of forming a yolk-shell structure with internal void space to tolerate the volume expansion of sulfur during discharge was proposed by Cui et al. [13,23,31] and the composites exhibited distinctly improved cycling performance (>1000 cycles). Though these new cathode materials shed a light on LieS battery research, the actual progress was far insufﬁcient for practical application. For example, in these studies the sulfur loading density was less than 1 mg cm2 [32e38]. In this case the theoretical overall cathode capacity per unit area is about 60% of that of LiCoO2 cathode in a commercial Li-ion batteries and the energy density is merely about 35% due to the lower working voltage of LieS system. To compete with lithium-ion batteries using LiCoO2 electrode, one would need a minimum sulfur loading density of 3 mg cm2 in the cathode. Some high sulfur loading density cases have been reported [39e42]; however, a high sulfur loading density often associates with mechanical failure of the electrode ﬁlm, e.g. cracking and/or peeling, leading to poor battery performance. It remains a challenge to develop high quality sulfur electrode for high performance LieS batteries. Apart from cathode materials, the selection of electrolyte is crucial for LieS batteries . The electrolyte is the media that transports lithium ions and dissolves polysulﬁdes (PS) which signiﬁcantly impacts the overall electrochemical performances of LieS battery . Electrolyte with low viscosity and high PS solubility generally favors the cell reaction; however, the dissolution of PS imposes negative impact on coulombic efﬁciency and capacity retention. Such negative impact can be suppressed by the introduction of LiNO3 additive into the electrolyte . During the discharge process, sulfur is gradually reduced to soluble PS (Li2S8, Li2S6 and Li2S4). Li2S4 is further reduced to insoluble sulﬁdes (Li2S2 and Li2S) that precipitate on the carbon surface at the end of discharge. In the reversed charge process, insoluble PS is ﬁrst oxidized into soluble PS which is further converted into sulfur and eventually precipitates on the carbon surface when charge is completed. The excess amount of PS in the electrolyte may cover the sulfur surface as a nonconductive coating and adversely impact the following discharge performance. Moreover, the amount of electrolyte also affects the cell performance. Larger volume of electrolyte generally leads to a higher initial discharge capacity ; however, it reduces the energy density of the cell. Therefore, it is critical to balance the volume of electrolyte and the amount of sulfur for high performance LieS batteries. In this work, we prepared a series of carbon/sulfur (C/S) composites with a different weight ratio (3:1, 2:1, 1:1, 1:2 and 1:3) and evaluated their electrochemical performances in LieS batteries. A high sulfur content and crack-free electrode with a loading density of 10 mg cm2 was fabricated, as carbon black was substituted by
ﬁne graphite powders. The effect of the volume of electrolyte on the electrochemical performances was also investigated. 2. Experimental C/S composites were prepared by manually mixing carbon black (Denka) or synthetic graphite (KS-6, TIMREX®) with precipitated sulfur (99.5%, Alfa Aesar) in different weight ratios in an agate mortar. The mixture of C/S composite (95 wt.%) and poly(vinylidene ﬂuoride) (PVDF, Solef® 5130, 5 wt.%) was dispersed in 1-methyl-2pyrrolidinone (NMP) to form a slurry which was subsequently casted onto Al foil as a current collector. After drying for 2 h in air at 80 C, electrode discs of 15 mm in diameter were punched out (without pressing) and transferred into an argon-ﬁlled glovebox (MBraun) for assembly. The electrolyte used was 1 M lithium bis(tri-ﬂuoromethanesulfonyl)imide (LiTFSI) in solvent mixture of 1,2-Dimethoxyethane (DME) and 1,3-Dioxolane (DOL) (v/v, 1:1) with 0.725 mol L1 of lithium nitrate (LiNO3) as additive. LieS coin cells (CR2032) were assembled with Li metal as counter electrode. One pair of wave spring and spacer was used to make the cell fullﬁlled. The cathode and Li anode were separated by an Asahi separator with a thickness of 16 mm. The cells were tested on a multichannel battery tester (Shenzhen Neware Co. Ltd.) at a constant current of 0.1 mA. The cycling voltage range was between 1.5 and 3.2 V (all the voltage mentioned in this work is vs. Liþ/Li). 3. Results and discussion 3.1. Optimization of carbonesulfur ratio As sulfur exists in its allotrope of octasulfur (cyclo-S8), the S8 rings are opened during the discharge and some of the resultant S8 chains are further cut shorter. Subsequently, these sulfur with different chain lengths are reduced to a series of Li2Sn (n ¼ 4e8) which are soluble in electrolyte, exhibiting a voltage slope at 2.3 V. Theoretically this step is anticipated to deliver a speciﬁc capacity of 418 mA h g1-sulfur; however, in practice the capacity is often affected by incomplete utilization of sulfur, especially if the sulfur particle size is too big. In the followed step, soluble Li2Sn are further reduced to form insoluble Li2S2 and Li2S as precipitate on carbon matrix, leading to a long voltage plateau at 2.1 V. This process delivers a theoretical speciﬁc capacity of 1254 mA h g1-sulfur. Assuming that sulfur was fully converted into Li2Sn in the ﬁrst step, the capacity at the second step should be mainly inﬂuenced by the property of the carbon matrix. Generally, larger surface area accommodates more Li2S2 and Li2S precipitates, and higher conductivity allows for easier conversion of Li2S2 to Li2S. It is noteworthy here that the cycling performance of LieS batteries can be affected by the nucleation and growth of Li2S2/Li2S . As the cell was further discharged to 1.5 V, another slope at 1.7 V from the reduction of LiNO3 appeared . The electrolyte additive, LiNO3, is used to stabilize Li anode by the formation of an enhanced solid electrolyte interface (SEI) ﬁlm, which can improve the coulombic efﬁciency of LieS batteries . As sulfur has poor electronic conductivity, it needs to be blended or combined with a conductive agent, e.g. carbon black, to form C/S composites as working cathode. High sulfur content in the C/S composite favors high energy density; however, too low carbon content will lead to the formation of electrically isolated islands in the electrode. Consequently, the sulfur utilization rate will be low (affecting the capacity delivered at 2.3 V), and so does the subsequent precipitation of soluble Li2Sn (causing capacity loss at the voltage plateau of 2.1 V). It is thus crucial to have a balanced carbon to sulfur ratio in the C/S composite cathode. As for the carbon sources, some recent work reported carbon black as a good
N. Ding et al. / Journal of Power Sources 269 (2014) 111e116
candidate for LieS batteries . The performance of batteries using electrode of C/S composites with different ratio of Denka black to sulfur is shown in Fig. 1a. As expected, at the C/S ratio of 1:3 (high sulfur content), the speciﬁc capacity was about 466 mA h g1sulfur which is only about 27.9% of the theoretical value (1672 mA h g1-sulfur). Table 1 summarizes the capacities attributed to the tree cell reactions discussed above for C/S composites with different C/S ratio. It is clearly seen that for the composite with a C/S ratio of 1:3, 62.7% of sulfur was reduced to Li2Sn (262 mA h g1-sulfur in experiment vs 418 mA h g1-sulfur in theory), and the conversion of Li2Sn to Li2S after fully discharged was as low as 13.9% (174 mA h g1-sulfur in experiment vs 1254 mA h g1-sulfur in theory). Such low conversion is likely due to the unavailability of sufﬁcient carbon surface that can accommodate the precipitation of Li2S2 and Li2S. This hypothesis is veriﬁed when the C/S ratio was increased from 1:3 to 1:2, where a 2 times of capacity increase is seen from the step of Li2Sn reduction to Li2S (538 mA h g1-sulfur vs 174 mA h g1-sulfur). As the C/S ratio was further increased to 1:1, the sulfur utilization rate at ﬁrst reduction plateau increases to 78.5% (328 mA h g1-sulfur vs 418 mA h g1-sulfur) and more capacity was delivered by the reduction reaction of Li2Sn (758 mA h g1-sulfur vs 538 mA h g1sulfur). At the carbon content of 50 wt% and higher, the capacities from the reduction of cyclo-S8 to soluble Li2Sn and from the reduction of Li2Sn to Li2S started to decrease slowly. This may be due to the increased self-discharge reaction and the precipitation of
Table 1 Summary of the capacities derived from each step of cell reactions in LieS batteries. C/S ratio
Capacity delivered at the plateau of 2.3 V (mA h g1-sulfur)
Capacity delivered at the plateau of 2.1 V (mA h g1-sulfur)
Capacity resulted from the reduction of LiNO3 (mA h)a
1:3 1:2 1:1 2:1 3:1 Theoretical value
262 312 328 303 300 418
174 538 758 660 656 1254
0.07 0.09 0.12 0.28 0.30 0.78
a The capacity is calculated LiNO3 þ 2Liþ þ 2e / LiNO2 þ Li2O.
Li2S on Li anode. In general, self-discharge rate of LieS batteries is higher than that of Li-ion batteries due to the existence of PS redox shuttle that reacts with Li to form precipitates on the anode. This phenomenon is even more pronounced for the samples with higher C/S ratios. Typically, loading of C/S composites in electrode was 1.7 mg cm2 in this work. In this case, sulfur is insufﬁcient to compensate the loss due to its precipitation onto the Li anode. In addition, a long voltage slope is observed at 1.7 V for the composite with high carbon content which is attributed to the reduction of LiNO3 on carbon matrix (LiNO3 þ 2Liþ þ 2e / LiNO2 þ Li2O). Such reduction is irreversible in the voltage window of 1.5e3.2 V, leading to the formation of a stable passivation layer on the carbon matrix. This is conﬁrmed by the disappearance of the voltage slope at 1.7 V in the following cycles. Fig. 1b presents the relationship between C/ S ratio and speciﬁc capacity (per gram electrode, including sulfur, carbon and binder) in 2nd cycle. A maximum capacity of 538 mA h g1-electrode was achieved for the composite with C/S ratio of 1:2, which is 3 times higher than that of LiCoO2 cathode (130 mA h g1-electrode, assuming with 5 wt% of PVDF binder). Thus, 1:2 was used as the carbon to sulfur ratio in the further optimization experiments. 3.2. Effects of sulfur loading and electrolyte volume on the electrode speciﬁc capacity Active material loading in electrode signiﬁcantly impacts the energy density of an electrode. In a commercial Li-ion battery, the
Fig. 1. LieS battery performance of C/S composites with varied ratio of carbon black to sulfur: (a) voltage proﬁles in the ﬁrst 5 cycles and (b) the relationship between electrode capacity (2nd cycle) and C/S ratio. The loading density of C/S composite was 1.7 mg cm2 and the volume of electrolyte used was 20 mL. The applied current density is 56.6 mA cm2.
Fig. 2. Initial discharge voltage proﬁles of the C/S composite (C:S ¼ 1:2) with different sulfur loading density (mg cm2) and the volume of electrolyte used was 20 mL. The applied current density is 56.6 mA cm2.
N. Ding et al. / Journal of Power Sources 269 (2014) 111e116
Fig. 3. Electrochemical performance of the C/S composite (C:S ¼ 1:2) cycled in different volume of electrolyte: (a) initial discharge voltage proﬁles and (b) cycling performance. The sulfur loading density was 2.4 mg cm2 and The applied current density is 56.6 mA cm2.
energy density of LiCoO2 electrode is generally about 2.7 mA h cm2 which is higher than that of S/C electrode with a typical value of 1.1 mA h cm2. To improve the energy density of S/C electrode, one can increase loading of sulfur and/or thickness of electrode. In this work, thicker cathode ﬁlms were prepared from slurry consisting of C/S composite (with C/S ratio of 1:2) and PVDF
binder onto aluminum foils using doctor-blade casting. The discharge curves for S/C composite cathodes of different sulfur loading are displayed in Fig. 2. One can see that as the sulfur loading was increased from 1.2 to 2.4 mg cm2, the capacity per unit mass of sulfur was reduced by 45%e459 mA h g1-sulfur. This is likely caused by the incomplete conversion of Li2Sn to Li2S, as concluded from a shorter voltage plateau at 2.1 V. Further increase of sulfur loading, e.g. to 3.0 mg cm2, led to a sharp capacity fade where the disappearance of the voltage plateau at 2.1 V suggested Li2Sn (n ¼ 6, 8) as the ﬁnal product of sulfur reduction in the discharge process. The partial reduction of sulfur may be attributed to the saturation of Li2S8/Li2S6 in the electrolyte, where these insoluble solids covered the unreacted sulfur and stopped further cell reaction. In this context, the volume of electrolyte also plays an important role in the capacity of the cell. Generally, larger volume of electrolyte helps dissolve more PS during discharge and also better wet the electrode; however, the brought-in drawback is the decrease of the energy density. The effect of the electrolyte volume on the initial discharge voltage proﬁles of S/C composite cathodes was investigated, and the results are shown in Fig. 3a. It can be seen that as the electrolyte volume was increased from 20 to 40 mL, the capacity increases by 71 mA h g1-sulfur (cf. total changes from the voltage plateaus at 2.3 and 2.1 V). Such synchronous increase of cell capacities at two plateaus seems to indicate improved wetting of the electrode. As the electrolyte volume was further increased to 80 mL, the increase of capacity at 2.3 V was signiﬁcantly slowed down (288 mA h g1sulfur). Interestingly, more Li2Sn were converted into Li2S2/Li2S at the end of discharge which delivered a doubled capacity as 575 mA h g1-sulfur at 2.1 V. Furthermore, a clear voltage slope was observed which can be attributed to the reduction of LiNO3. With sulfur loading of 2.4 mg cm2 and electrolyte volume of 80 mL, a capacity of 1066 mA h g1-sulfur was delivered by the electrode. The initial capacity per square centimeter in this case can be as high as 2.8 mA h cm2. Nevertheless, increasing electrolyte volume is by no means a good way for the improvement of LieS battery performance. Not only will the energy density drop at cell level, but also poor cell cyclic stability is rendered. This can be clearly seen from the testing results of a number of cells with different electrolyte volume, ranging from 20 to 80 mL, as shown in Fig. 3b. For LieS cells with 20 and 40 mL of electrolyte, almost constant capacities of 550 and 600 mA h g1-sulfur are seen in the ﬁrst 25 cycles. As a clear contrast, the cell with 80 mL of electrolyte showed a large initial capacity loss (119 mA h g1-sulfur). This could be due to the leftover of Li2S6 and Li2S4 in the electrolyte at the end of discharge . Larger volume of electrolyte may work as a PS reservoir in the cell and also accelerates the PS transport from
Fig. 4. Deformability test of electrodes (C:S ¼ 1:2) prepared with carbon black and KS-6, with a sulfur loading density of 10 mg cm2.
N. Ding et al. / Journal of Power Sources 269 (2014) 111e116
3.3. Improvement of bonding performance The fast capacity fading of the cell with large volume of electrolyte suggests the need of even higher sulfur loading density on cathode current collector to improve the energy density; however, thicker ﬁlms from composite of sulfur and carbon black of high surface area are brittle and tend to peel off from the current collector, as shown in Fig. 4. This situation is signiﬁcantly improved by replacing carbon black with conductive ﬁne graphite powders (KS6). With KS-6 the sulfur loading density can be as high as 10 mg cm2 and the electrode ﬁlm shows good mechanical properties for wrapping and pressing. The initial discharge voltage proﬁles of KS-6/sulfur composite (C:S ¼ 1:2) with varied sulfur loading density are shown in Fig. 5a. A volume of 80 mL of electrolyte was universally used to ensure completely wetted electrodes. At sulfur loading density of below 4.5 mg cm2, a similar capacity in the range of 612e688 mA h g1sulfur was delivered. As sulfur loading density was increased to 5.8 mg cm2, the capacity dropped to 440 mA h g1-sulfur. With further increasing the sulfur loading density to 10 mg cm2, the cell can only retain a capacity of 197 mA h g1-sulfur. The corresponding areal capacities at varied sulfur loading density are calculated to be 0.76 (1.1 mg cm2), 1.35 (2.0 mg cm2), 2.17 (3.5 mg cm2), 2.77 (4.5 mg cm2), 2.55 mA h cm2 (5.8 mg cm2), 2.03 mA h cm2 (8.2 mg cm2) and 1.97 mA h cm2 (10.0 mg cm2) respectively (Fig. 5b). With sulfur loading density of 4.5 mg cm2 the power density of the electrode reached 5.88 mW h cm2. Using the KS-6/S composites on electrodes leads to 58e63% of capacity loss in comparison to their counterparts using carbon black/S composites; however, good cyclic performance is observed (Fig. 5c). Lower capacities of KS-6/sulfur composites are also seen in the shortened voltage plateau at 2.1 V, which is likely attributed to the lower surface area of KS-6 (affects the extent of Li2S4 to Li2S2/Li2S conversion). Introduction of additional carbon materials with large surface area that helps provide more precipitation sites for Li2Sn, e.g. activated carbon, may be the solution to compensate the capacity loss caused by the use of KS-6/sulfur composite. 4. Conclusions The performance of a LieS battery is affected by multiple parameters. Electrolyte volume, carbon/sulfur ratio and sulfur loading density, as well as the choice of carbon source impact the battery performance in terms of capacity, cycleability, and processibilities. The C/S composite may deliver a capacity of 538 mA h g1-electrode which is 3 times as high as that of LiCoO2. The capacity per square centimeter can be improved with higher sulfur loading density. Sulfur loading density can be further increased by replacing carbon black with ﬁne graphite powders. With these optimizations the electrode delivers a power density of 5.88 mW h cm2 which is 60% of the commercial LiCoO2 electrode. Fig. 5. (a) Initial discharge voltage proﬁles, (b) the curve of areal capacity vs. sulfur loading density and (c) cycling performance of the KS-6/sulfur composite (C:S ¼ 1:2) with different sulfur loading density (mg cm2). The volume of electrolyte used was 80 mL and the applied current density is 56.6 mA cm2.
cathode to Li anode, giving rise to a fast capacity fading. Such fast capacity drop in the ﬁrst a few cycles is often seen in the study of LieS batteries [13,31,40,41] which however can be suppressed if the carbon microstructure is modiﬁed to be better PS absorbent . The optimization of the ratio between sulfur and liquid electrolyte has been systematically investigated and reported recently by Zheng et al. .
Acknowledgments This research was supported by the Advanced Energy Storage Research Programme (IMRE/12-2P0503 and IMRE/12-2P0504), Institute of Materials Research and Engineering (IMRE) of the Agency for Science, Technology and Research (A*STAR), Singapore. References  J.M. Tarascon, M. Armand, Nature 414 (2001) 359e367.  J.B. Goodenough, Y. Kim, Chem. Mater. 22 (2010) 587e603.  F. Leroux, G. Goward, W.P. Power, L.F. Nazar, J. Electrochem. Soc. 144 (1997) 3886e3895.  J. Liu, H. Xia, D. Xue, L. Lu, J. Am. Chem. Soc. 131 (2009) 12086e12087.
N. Ding et al. / Journal of Power Sources 269 (2014) 111e116
 Y. Wang, G.Z. Cao, Chem. Mater. 18 (2006) 2787e2804.  X. Feng, N. Ding, Y. Dong, C. Chen, Z. Liu, J. Mater. Chem. A 1 (2013) 15310e15315.  A. Debart, J. Bao, G. Armstrong, P.G. Bruce, J. Power Sources 174 (2007) 1177e1182.  X. Ji, L.F. Nazar, J. Mater. Chem. 20 (2010) 9821e9826.  C.P. Yang, S. Xin, Y.X. Yin, H. Ye, J. Zhang, Y.G. Guo, Angew. Chem. Int. Ed. 52 (2013) 8363e8367.  S.S. Zhang, J. Power Sources 231 (2013) 153e162.  P.G. Bruce, S.A. Freunberger, L.J. Hardwick, J.M. Tarascon, Nat. Mater. 11 (2012) 19e29.  W.J. Chung, J.J. Griebel, E.T. Kim, H. Yoon, A.G. Simmonds, H.J. Ji, P.T. Dirlam, R.S. Glass, J.J. Wie, N.A. Nguyen, B.W. Guralnick, J. Park, A. Somogyi, P. Theato, M.E. Mackay, Y.E. Sung, K. Char, J. Pyun, Nat. Chem. 5 (2013) 518e524.  Z.W. Seh, W. Li, J.J. Cha, G. Zheng, Y. Yang, M.T. McDowell, P.C. Hsu, Y. Cui, Nat. Commun. 4 (2013) 1331.  G. Zhou, S. Pei, L. Li, D.W. Wang, S. Wang, K. Huang, L.C. Yin, F. Li, H.M. Cheng, Adv. Mater. 26 (2014) 625e631.  G. Zheng, Q. Zhang, J.J. Cha, Y. Yang, W. Li, Z.W. Seh, Y. Cui, Nano Lett. 13 (2013) 1265e1270.  N. Jayaprakash, J. Shen, S.S. Moganty, A. Corona, L.A. Archer, Angew. Chem. Int. Ed. 50 (2011) 5904e5908.  J. Zheng, J. Tian, D. Wu, M. Gu, W. Xu, C. Wang, F. Gao, M.H. Engelhard, J.G. Zhang, J. Liu, J. Xiao, Nano Lett. 14 (2014) 2345e2352.  S. Xin, L. Gu, N.H. Zhao, Y.X. Yin, L.J. Zhou, Y.G. Guo, L.J. Wan, J. Am. Chem. Soc. 134 (2012) 18510e18513.  J.T. Lee, Y. Zhao, S. Thieme, H. Kim, M. Oschatz, L. Borchardt, A. Magasinski, W.I. Cho, S. Kaskel, G. Yushin, Adv. Mater. 25 (2013) 4573e4579.  J. Schuster, G. He, B. Mandlmeier, T. Yim, K.T. Lee, T. Bein, L.F. Nazar, Angew. Chem. Int. Ed. 51 (2012) 3591e3595.  L. Ji, M. Rao, H. Zheng, L. Zhang, Y. Li, W. Duan, J. Guo, E.J. Cairns, Y. Zhang, J. Am. Chem. Soc. 133 (2011) 18522e18525.  G. He, S. Evers, X. Liang, M. Cuisinier, A. Garsuch, L.F. Nazar, ACS Nano 7 (2013) 10920e10930.  W. Li, G. Zheng, Y. Yang, Z.W. Seh, N. Liu, Y. Cui, Proc. Natl. Acad. Sci. U. S. A. 110 (2013) 7148e7153.  J. Gao, H.D. Abruna, J. Phys. Chem. Lett. 5 (2014) 882e885.  X. Ji, K.T. Lee, L.F. Nazar, Nat. Mater. 8 (2009) 500e506.  J. Jin, Z. Wen, G. Ma, Y. Lu, Y. Cui, M. Wu, X. Liang, X. Wu, RSC Adv. 3 (2013) 2558e2560.  H. Wang, Y. Yang, Y. Liang, J.T. Robinson, Y. Li, A. Jackson, Y. Cui, H. Dai, Nano Lett. 11 (2011) 2644e2647.
 J. Guo, Y. Xu, C. Wang, Nano Lett. 11 (2011) 4288e4294.  L. Yuan, H. Yuan, X. Qiu, L. Chen, W. Zhu, J. Power Sources 189 (2009) 1141e1146.  M.Q. Zhao, X.F. Liu, Q. Zhang, G.L. Tian, J.Q. Huang, W. Zhu, F. Wei, ACS Nano 6 (2012) 10759e10769.  W. Zhou, Y. Yu, H. Chen, F.J. DiSalvo, H.D. Abruna, J. Am. Chem. Soc. 135 (2013) 16736e16743.  W. Weng, V.G. Pol, K. Amine, Adv. Mater. 25 (2013) 1608e1615.  J.T. Lee, Y. Zhao, H. Kim, W.I. Cho, G. Yushin, J. Power Sources 248 (2014) 752e761.  S. Moon, Y.H. Jung, W.K. Jung, D.S. Jung, J.W. Choi, D.K. Kim, Adv. Mater. 25 (2013) 6547e6553.  Y. Yang, G. Yu, J.J. Cha, H. Wu, M. Vosgueritchian, Y. Yao, Z. Bao, Y. Cui, ACS Nano 5 (2011) 9187e9193.  G. Zheng, Y. Yang, J.J. Cha, S.S. Hong, Y. Cui, Nano Lett. 11 (2011) 4462e4467.  G. He, X. Ji, L. Nazar, Energy Environ. Sci. 4 (2011) 2878e2883.  L.L. Peng, G.B. Liu, Y. Wang, Z.L. Xu, H. Liu, J. Solid State Electrochem. 18 (2014) 935e940.  J. Song, T. Xu, M.L. Gordin, P. Zhu, D. Lv, Y.B. Jiang, Y. Chen, Y. Duan, D. Wang, Adv. Funct. Mater. 24 (2014) 1243e1250.  T. Xu, J. Song, M.L. Gordin, H. Sohn, Z. Yu, S. Chen, D. Wang, ACS Appl. Mater. Interfaces 5 (2013) 11355e11362.  L.X. Miao, W.K. Wang, A.B. Wang, K.G. Yuan, Y.S. Yang, J. Mater. Chem. A 1 (2013) 11659e11664.  S.S. Zhang, Electrochem. Commun. 31 (2013) 10e12.  J. Zheng, M. Gu, H. Chen, P. Meduri, M.H. Engelhard, J.-G. Zhang, J. Liu, J. Xiao, J. Mater. Chem. A 1 (2013) 8464e8470.  S.S. Zhang, Energies 5 (2012) 5190e5197.  Y.V. Mikhaylik, U.S. Patent (2008) 7,352,680.  S. Urbonaite, P. Novak, J. Power Sources 249 (2014) 497e502.  J. Zheng, M. Gu, C. Wang, P. Zuo, P.K. Koech, J.-G. Zhang, J. Liu, J. Xiao, J. Electrochem. Soc. 160 (2013) A1992eA1996.  S.S. Zhang, Electrochim. Acta 70 (2012) 344e348.  D. Aurbach, E. Pollak, R. Elazari, G. Salitra, C.S. Kelley, J. Afﬁnito, J. Electrochem. Soc. 156 (2009) A694eA702.  J. Zheng, M. Gu, M.J. Wagner, K.A. Hays, X. Li, P. Zuo, C. Wang, J.-G. Zhang, J. Liu, J. Xiao, J. Electrochem. Soc. 160 (2013) A1624eA1628.  Y. Diao, K. Xie, S. Xiong, X. Hong, J. Electrochem. Soc. 159 (2012) A421eA425.  J. Zheng, D. Lv, M. Gu, C. Wang, J.-G. Zhang, J. Liu, J. Xiao, J. Electrochem. Soc. 160 (2013) A2288eA2292.